The Influence of Implant Abutment Surface Roughness and the Type of Cement on Retention of Implant Supported Crowns
S. VARALAKSHMI REDDY 1, M. Sushender Reddy2, C. Rajaneesh Reddy3, Padmaja Pithani4, Santosh Kumar R5, Ganesh kulkarni6
ABSTRACT Objectives: To provide relative data on the retentive characters of the commonly used cements on different implant abutment surfaces. Materials and Methods: A total of 20 implant abutments were divided into 2 groups. Ten implants were unaltered and ten were air borne particle abraded with 50µ aluminium oxide. Three luting agents (Tempbond, IRM and ImProv) were used to secure the crowns to abutments. All the crowns were removed from the abutment with an Instron machine at 0.5mm per minute and tensile bond strengths were recorded. Statistical analysis was performed using Anova, Paired t-test and Post-Hoc tests.
Results: IRM showed the highest mean tensile strength among the three cements when used with treated and untreated implant abutment surfaces. Change in the abutment surface roughness had no effect on the mean tensile bond strength of TempBond and IRM cements, whereas ImProv cement showed reduced tensile strength with sandblasted surface. Conclusion: When increased retention is required IRM cement with either sandblasted or milled surface could be used and when retrievability is required cements of choice could be either TempBond or ImProv.
Keywords: Aluminum oxide, Dental Cements, Eugenol, Methymethacrylates, Tensile strength
Introduction Implants have revolutionized the dental practice in the last few decades. They are being considered as a better alternative to conventional fixed or removable prosthesis as they have overcome many of the limitations encountered with these conventional approaches. Implant supported prostheses are considered as highly esthetic, functional restorations with long-term predictability . One of the most important decisions in implant prosthodontics is to choose between screw-retained and cement retained restorations . The choice between screw-retained and cement retained restorations has always been a controversy in the literature. It has been documented that screw retained restorations were successful in edentulous arches. However, they do have disadvantages such as, screw loosening and screw fracture . Cement retained prostheses have superior esthetics, easier control of occlusion, and are economical when compared to screw retained restorations but are not retrievable .The abutment preparation design and the cementation technique are similar to the conventional fixed procedures for natural teeth. So, all the factors that influence the retention in the restorations over natural teeth also affect the retention in implant supported crowns . The factors that can affect the retention are abutment taper, surface area, height, surface finish and roughness. By increasing the surface roughness of the implant abutment the retention of the cement retained restoration can be improved . The type of cement used is also an important factor in determining the retention of the restoration . Retention of the luted provisional implant restoration can be a challenge, especially as the provisional implant restoration should minimize micro movement that may interfere with implant osseointegration [5,6]. Improvement of the implant surfaces such as airborne-particle abrasion and acid etching make early or immediate loading more successful. The values for the retentive strength for the different classes of luting cements are reported in the literature [7-14]. The Journal of Clinical and Diagnostic Research. 2015 Mar, Vol-9(3): ZC05-ZC07
choice of cement for an implant supported restoration should be based on the need or desire for retrievability, the anticipated amount of retention needed, removal and cost [12-17].The aim of this study is to provide relative data on the retentive characters of the commonly used cements on different implant surfaces.
MATERIALS AND METHODS Impressions of the implant abutments were made and casts were poured [Table/Fig-1]. Wax patterns were fabricated by dipping technique (waxpot) to provide 0.5 mm thick standard wax patterns [17,18] and a sprue of uniform length of 3mm was attached to the wax pattern. Wax patterns were then invested in a phosphate bonded investment and casting was done using nickel chromium alloy. Burnout casting procedure was followed according to the manufacturer’s instructions and the castings were divested. The remnants of investment on the surface of the abutment were removed by the use of sandblaster with the use of 50 microns aluminium oxide. After sand blasting, the samples were ultrasonically cleaned for 3 min in a distilled waterbath. Finally 60 specimens were divided into 2 groups of 30 each. Each group was sub divided into 3 subgroups of 10 samples each. Group I: Control group. Group II: Sandblasting group An abrasive tool with 50 micron aluminium oxide particles with a pressure of 5 kg/cm2 at a distance of 5 mm away from the surface with a circulating motion at 6 mm in diameter for 20 seconds was used to abrade the abutment surface. After sandblasting, the specimens were ultrasonically cleaned for 15 mins in distilled water. Autopolymerising acrylic resin blocks were fabricated, allowing the implant analogs to be placed in the blocks perpendicular to the face 5
S. VaraLakshmi Reddy et al., Factors Influencing Retention in Implant Crowns
of the resin block. The abutments were connected to the implant analogs and torqued to 35 N-cm. After fabrication of 3 cast crowns for each abutment the luting agent Tempbond, ImProv and IRM cements were used to secure the crowns to respective abutments [Table/Fig-2]. All specimens were stored in 100% humidity for one day at 37oC prior to testing. Each crown was removed from the abutment with an Instron mechanical testing machine at 0.5mm/ min  and the tensile strength was recorded.
[Table/Fig-1]: Study samples [Table/Fig-2]: Cements used in the study
RESULTS When Group I (control) specimens were luted with type A (IRM), typeB (TempBond cement) and type C (ImProv cement), the mean tensile bond strengths were 258.28N, 138.41N and 184.86N respectively.When Group II (sandblasted) specimens were luted with type A (IRM), type B (TempBond cement) and type C (ImProv cement), the mean tensile bond strengths were 260.68N, 138.28N and 152.13N respectively [Table/Fig-3-5]. Both type A and B did not show any significant differences in tensile strength between the control and sandblasted surfaces whereas type C showed an increase in the tensile bond strength with the Group I samples (control) when compared to Group II samples. N
Std. Error Mean
[Table/Fig-3]: Mean tensile bond strength of Type A cement with Group I and II-Paired Samples Statistics N
Std. Error Mean
Control Temp Bond
Sandblasted Temp Bond
[Table/Fig-4]: Mean tensile bond strength of Type B cement with Group I and II-Paired Samples Statistics N
Std. Error Mean
[Table/Fig-5]: Mean tensile bond strength of Type C cement with Group I and II-Paired Samples Statistics
Statistical analysis Paired t-test was used to compare the mean tensile bond strength values between the three luting agents among the two groups. The mean tensile strength values of Group I and Group II did not show any statistically significant differences when tested with type A and type B cements(p>0.5). However, there was a decrease in the mean tensile bond strength value with Type C cement in the sandblasted group by 17%, which was statistically significant (p0.5). In sub-group B also the mean tensile strength of group I (control) was 138.41N and Group II (sandblasted) was 138.20N. The differences between the mean tensile strength were also not statistically significant (p-value>0.5). Few other studies indicate that the effect of interaction between the surface characteristics and luting agent affect the tensile bond strength. This surface alteration could be done either with the use of rotary instruments or sand blasting. In a study done by Yongsik Kim , there were no differences in the tensile strength of TempBond and other provisional luting agents when used with all different surface conditions. In another study done by Wolfart M  retention of the castings cemented with eugenol free zinc oxide cements was not affected by abutment surface conditioning by air abrasion. According to DJ Witwer , rough finished surfaces showed a significantly (p